1. Introduction {#sec1-materials-10-00477}
===============

Magnesium-based alloys have aroused keen attention as biodegradable bone implants due to their unique biodegradable characteristics, proper mechanical properties and favorable biocompatibility \[[@B1-materials-10-00477],[@B2-materials-10-00477],[@B3-materials-10-00477],[@B4-materials-10-00477],[@B5-materials-10-00477],[@B6-materials-10-00477]\]. The widely used Mg-Al-Zn (AZ series) alloys belong to a magnesium-based alloy, which exhibits high strength and certain degradation resistance \[[@B7-materials-10-00477],[@B8-materials-10-00477],[@B9-materials-10-00477],[@B10-materials-10-00477]\]. Nevertheless, it still needs to further enhance degradation resistance in order to have biological applications \[[@B11-materials-10-00477],[@B12-materials-10-00477],[@B13-materials-10-00477]\]. The rare earth elements such as neodymium (Nd), gadolinium (Gd) and yttrium (Y) have a beneficial effect in increasing degradation resistance and enhance the mechanical properties of magnesium alloys \[[@B14-materials-10-00477],[@B15-materials-10-00477],[@B16-materials-10-00477],[@B17-materials-10-00477],[@B18-materials-10-00477]\].

Many research works have been carried out on magnesium alloys with rare earth elements. Zhang et al. \[[@B19-materials-10-00477]\] reported that alloying cerium (Ce) could improve mechanical properties and corrosion resistance of cast Mg-4Al-based alloy. Liu et al. \[[@B20-materials-10-00477]\] reported that the addition of Lanthanum (La) could enhance the corrosion properties of AM60 alloy. Yttrium (Y), a rare earth element, has hexagonal close-packed crystal structure which is the same as that of magnesium, and the atomic radius of Y (0.18 nm) is close to that of magnesium (0.16 nm) \[[@B21-materials-10-00477]\]. Thus, its solid solubility limit in magnesium alloys can reach up to 11.4 wt % \[[@B22-materials-10-00477]\]. Moreover, Y has the same standard electrochemical potential with magnesium (−2.372 V) \[[@B23-materials-10-00477],[@B24-materials-10-00477]\]. Qi et al. investigated the effects of Y on the microstructure and mechanical properties of as-cast Mg-6Zn-1Mn alloy. The results showed that Y could improve its mechanical properties significantly, and the alloy with Y content of 6.09 wt % has the best mechanical properties \[[@B25-materials-10-00477]\]. Luo et al. studied the corrosion resistance property and the corrosion evolution of as-cast AZ91 alloy with rare earth Y. They found that the proper amount of Y addition could improve the corrosion resistance of as-cast AZ91 alloys effectively \[[@B26-materials-10-00477]\].

Laser rapid melting has the characteristic of rapid solidification. The cooling rate during laser melting usually reaches up to 10^5^ K/s, which can inhibit grain growth and refine the grains \[[@B27-materials-10-00477]\]. Meanwhile, laser rapid melting can reduce the composition segregation. Furthermore, laser rapid melting is a non-equilibrium process which can increase the solid solubility of the alloy elements \[[@B28-materials-10-00477]\].

In this work, the AZ61 magnesium alloys (Mg-6Al-1Zn wt %) with different Y contents (0, 1, 2, 3, 4 wt %) were prepared using laser rapid melting. The microstructure was studied by optical microscopy (OM), X-ray diffraction (XRD) and scanning electron microscopy (SEM) with energy dispersed spectroscopy (EDS). The degradation properties were analyzed by the immersion experiments. In addition, the hardness was measured by Vickers hardness tests.

2. Results and Discussion {#sec2-materials-10-00477}
=========================

2.1. Microstructure {#sec2dot1-materials-10-00477}
-------------------

The microstructures of the AZ61 magnesium alloys with different amounts of Y added were examined by optical microscopy ([Figure 1](#materials-10-00477-f001){ref-type="fig"}) and scanning electron microscopy ([Figure 2](#materials-10-00477-f002){ref-type="fig"}) respectively. AZ61 magnesium alloy consisted of the magnesium matrix and network precipitates (pointed by black arrows) which were distributed mainly at grain boundaries ([Figure 1](#materials-10-00477-f001){ref-type="fig"}a and [Figure 2](#materials-10-00477-f002){ref-type="fig"}a). After adding Y, the network precipitates decreased and a small amount of granulous precipitates (pointed by black arrows with a round tail) appeared ([Figure 1](#materials-10-00477-f001){ref-type="fig"}b and [Figure 2](#materials-10-00477-f002){ref-type="fig"}b). The granulous precipitates increased as the Y contents increased and were distributed uniformly as Y reached 2 wt % ([Figure 1](#materials-10-00477-f001){ref-type="fig"}c and [Figure 2](#materials-10-00477-f002){ref-type="fig"}c). However, as the Y contents further increased, the granulous precipitates tended to be predominant and agglomerate ([Figure 1](#materials-10-00477-f001){ref-type="fig"}d,e and [Figure 2](#materials-10-00477-f002){ref-type="fig"}d,e).

The XRD patterns of the AZ61 magnesium alloys with different Y contents were exhibited in [Figure 3](#materials-10-00477-f003){ref-type="fig"}. Only the α-Mg and Mg~17~Al~12~ phase were detected in the AZ61 magnesium alloy ([Figure 3](#materials-10-00477-f003){ref-type="fig"}a). After adding Y, a new Al~2~Y phase was formed and the corresponding peak intensity gradually increased as Y increased. Meanwhile, the peak intensity of the Mg~17~Al~12~ phase decreased. This implied the reduction of the Mg~17~Al~12~ phase and the increase of the Al~2~Y phase. Reference intensity ratio (RIR) method was used to quantify the weight percent of the Mg~17~Al~12~ phase and Al~2~Y phase. A more complete view on the weight percent of the Mg~17~Al~12~ phase and Al~2~Y phase as influenced by Y content was given in [Figure 4](#materials-10-00477-f004){ref-type="fig"}. It could be observed that the weight percent of the Mg~17~Al~12~ phase decreased from 7.5% in the AZ61 magnesium alloy to 4.1% in the AZ61 magnesium alloy with 4 wt % Y, while that of Al~2~Y increased from 0% in the AZ61 magnesium alloy to 2.5% in the AZ61 magnesium alloy with 4 wt % Y. In general, the tendency of elements to form stable compounds was in positive correlation with the electronegativity difference between elements. The electronegativity values of Y, Mg and Al were 1.22, 1.31 and 1.61 respectively, from which it could be deduced that Y was prone to react with Al to form Al-Y compound \[[@B29-materials-10-00477]\]. Thus, the Al~2~Y phase increased gradually as Y increased, while the Mg~17~Al~12~ phase decreased.

The morphology and compositions of the second phases in AZ61 magnesium alloy with 2 wt % Y were studied by EDS. It was presented that magnesium content reduced while Al and Y increased across the granulous particles ([Figure 5](#materials-10-00477-f005){ref-type="fig"}b). Thus, it was reasonable to conclude that the granulous particle was in the Al~2~Y phase. Meanwhile, the rod-shaped phase had a Mg/Al ratio (78.78/21.22) ([Figure 5](#materials-10-00477-f005){ref-type="fig"}c) which was close to that of Mg~17~Al~12~, and was thereby identified as Mg~17~Al~12~ phase.

The three phases (α-Mg, Al~2~Y and Mg~17~Al~12~) were exactly determined in the AZ61 magnesium alloy with Y. The schematic diagram of the phase formation in the alloy was shown in [Figure 6](#materials-10-00477-f006){ref-type="fig"}. The first precipitated phase in the solidification of the high-temperature liquid phase was the Al~2~Y phase. This could be explained by the Al~2~Y phase having the highest melting point (1485 °C) among the three phases ([Figure 6](#materials-10-00477-f006){ref-type="fig"}b) \[[@B30-materials-10-00477]\]. Afterwards, the α-Mg phase with the melting point of 650 °C started nucleation ([Figure 6](#materials-10-00477-f006){ref-type="fig"}c). Then, the remained Al atoms precipitated in Mg~17~Al~12~ (437 °C) which distributed on the α-Mg grain boundaries ([Figure 6](#materials-10-00477-f006){ref-type="fig"}d).

2.2. Hardness {#sec2dot2-materials-10-00477}
-------------

The hardness of AZ61 magnesium alloys with different Y contents was shown in [Figure 7](#materials-10-00477-f007){ref-type="fig"}. The hardness of AZ61 magnesium alloy was 90.9 Hv. The hardness continuously increased as Y increased from 0 wt % to 2 wt %. The optimal hardness was 104.9 Hv when the Y content was 2 wt %. However, it decreased as the Y contents further decreased. The increase of hardness was attributed to the uniform distribution of Al~2~Y and Mg~17~Al~12~ phases which acted as a second phase strengthening agent in the alloy matrix. As the Y contents further decreased, the excessive Al~2~Y phase formed in the alloy tended to aggregate. Thus, the structure of the alloy became uneven and the hardness of the alloy decreased.

2.3. Degradation Properties {#sec2dot3-materials-10-00477}
---------------------------

Immersion tests were applied to study the degradation properties of AZ61 magnesium alloys with different Y contents. The hydrogen evolution volume varied with the immersion time, as shown in [Figure 8](#materials-10-00477-f008){ref-type="fig"}. The hydrogen evolution volume of the alloys increased rapidly in the early stages of immersion and then increased slowly, which indicated a reduction of degradation rate. The hydrogen evolution volume of AZ61 magnesium alloys with Y contents of 0, 1, 2, 3 and 4 wt % were 30.1 mL/cm^2^, 13.3 mL/cm^2^, 6.1 mL/cm^2^, 10.5 mL/cm^2^ and 18.1 mL/cm^2^ after immersion for 360 h, respectively. It was observed that the degradation rate reduced remarkably with adding Y up to 2 wt %, while a further increase of Y resulted in an increased degradation rate. The degradation rates of the AZ61 magnesium alloys with different Y contents were calculated according to mass loss test ([Figure 9](#materials-10-00477-f009){ref-type="fig"}). The results were consistent with that of hydrogen evolution analysis, which showed that AZ61 magnesium alloy with 2 wt % Y exhibited the lowest degradation rate (0.28 mm/year). The degradation rate of AZ61 magnesium alloy with 2 wt % Y was lower than the reported value of WE43 magnesium alloy (0.85 mm/year) \[[@B31-materials-10-00477]\].

The degradation morphology of the AZ61 magnesium alloys with different Y contents after immersion for 120 h was shown in [Figure 10](#materials-10-00477-f010){ref-type="fig"}. Obviously, the alloys were covered with a degradation product film which presented some cracks. The appearance of cracks was believed to be caused by the dehydration of the degradation product film after drying in ambient atmosphere. The AZ61 magnesium alloy exhibited a severely corroded surface with many cracks ([Figure 10](#materials-10-00477-f010){ref-type="fig"}a). After adding 1 wt % Y, the surface of the alloy presented relatively shallow cracks. When the Y contents was 2 wt %, the integrated degradation film without a crack formed, which implied that the degradation degree of the alloy was relatively low ([Figure 10](#materials-10-00477-f010){ref-type="fig"}c). As the Y contents further increased, the cracks of the degradation product film gradually increased ([Figure 10](#materials-10-00477-f010){ref-type="fig"}d,e).

It could be concluded that the appropriate addition of rare earth element Y could enhance degradation resistance of the AZ61 magnesium alloy. In general, the Mg~17~Al~12~ phase acted as the cathode with respect to the magnesium matrix, which facilitated the degradation of the AZ61 magnesium alloy \[[@B32-materials-10-00477]\]. After adding Y, Y reacted with Al to form the Al~2~Y phase, which reduced the amount of Mg~17~Al~12~ phase on the grain boundaries. Furthermore, the Al~2~Y phase has more active potential \[[@B33-materials-10-00477]\]. Thus, adding Y could suppress the galvanic corrosion of the alloys, which enhanced the degradation resistance. However, as the Y contents further increased, the excessive Al~2~Y phase accelerated galvanic corrosion, resulting in the increase of degradation rate.

3. Experimental Procedure {#sec3-materials-10-00477}
=========================

3.1. Materials Preparation {#sec3dot1-materials-10-00477}
--------------------------

The spherical AZ61 magnesium alloy powders were purchased from Tangshan Weihao Materials Co., Ltd. (Tangshan, China, average particle size 70 µm) and irregular-shaped Y powders were obtained from Shanghai Naiou Nano technology Co., Ltd. (Shanghai, China, average particle size 20 µm). The powder mixtures with different Y contents (0, 1, 2, 3 and 4 wt %) were prepared through ball milling in a mixed gas environment (1 vol % SF~6~ and 99 vol % CO~2~). The rotation speed was fixed at 450 rpm (revolution per minute) in the course of ball milling and the milling time was 2 h.

The AZ61 magnesium alloys with different Y contents (0, 1, 2, 3, 4 wt %) were prepared using a homemade laser rapid melting system. It consists of a fiber laser, a focus system, a gas protection device and a computer control system. The fiber laser has a maximum output power of 110 W. The minimum spot diameter of the laser beams is 50 μm. More details of the system are available in the reference \[[@B34-materials-10-00477]\]. The processing parameters were as follows: laser scanning rate 200 mm/min, laser spot 150 μm and laser power 80 W. The powder mixtures were melted layer by layer in the sealed building chamber protected by argon gas. Then, the samples of alloys (10 mm × 10 mm × 5 mm) were built up.

3.2. Materials Characterization {#sec3dot2-materials-10-00477}
-------------------------------

The prepared alloy specimens were ground with abrasive papers grading from 1000 to 2000 grit and mechanically polished on cotton cloth with 0.5 μm diamond paste, followed by being etched for 10 s with the acetic picral solution (10 mL of acetic acid, 70 mL of ethanol (99.8% *v*/*v*), 4.2 g of picric acid, and 10 mL of distilled water), then the metallurgical structure of alloys was studied by an optical microscopy (OM, Olympus BHM, Osaka, Japan). The composition distribution of the alloys was studied using scanning electron microscopy (SEM, QUANTA FEG250, FEI Company, Hillsboro, OR, USA) and energy dispersive spectroscopy (EDS, JSM-5910LV, JEOL, Tokyo, Japan). The phase compositions were analyzed through X-ray diffraction (XRD, D8 Advance, Bruker Inc., Karlsruhe, Germany) using Cu-Kα radiation at 15 mA and 30 kV with scattering angles ranging from 10° to 80°, step size 0.02° and scanning speed 8°/min. X-ray diffraction patterns were identified by comparing the diffraction patterns with the standard ICDD-PDF cards. The quantitative phase analysis was conducted by means of the reference intensity ratio method \[[@B35-materials-10-00477]\].

Vickers hardness tests were performed by a Vickers microindenter (HXD-1000TM/LCD, Digital Micro Hardness Tester, Shanghai Taiming Optical Instrument Co. Ltd, Shanghai, China) with a load of 2.45 N and loading time of 15 s. Ten indents were made for each sample. The hardness was expressed as a mean and standard deviation of these 10 readings. The dimensions of alloys used for the immersion tests were 10 mm × 10 mm × 5 mm. Immersion tests were operated at 37 ± 0.5 °C in simulated body fluid (SBF) (the ratio of the surface area to solution volume was 1 cm^2^:100 mL). The SBF that has similar ion concentrations to those of human blood plasma was prepared according to the protocol described by Kokubo et al. \[[@B36-materials-10-00477]\]. In short, the relevant reagent grade chemicals (CaCl~2~, K~2~HPO~4~·3H~2~O, KCl, NaCl, MgCl~2~·6H~2~O, NaHCO~3~ and Na~2~SO~4~) were dissolved in distilled water at the appropriate amounts. The pH of the solution was buffered to physiological pH (pH = 7.4) by adding tri-hydroxymethyl-aminomethane and hydrochloric acid. The hydrogen evolution volume was monitored during the immersion. After immersion for 7 days, each sample was removed from the solution and washed with distilled water. A chromic acid solution (200 g/L Cr~2~O~3~ + 10 g/L AgNO~3~) was used to remove the degradation products on the sample surface before mass loss measurement. Five samples were measured for each group to obtain reproducible results. The degradation rates (mm/year) were calculated according to mass loss test. After immersion for 120 h, the samples were taken out from SBF and then blown dry with air at room temperature. The degraded surfaces were observed by SEM. Before the SEM observations, the samples were coated with gold by using a sputter coater (Leica EM SCD005, Leica Microsystems GmbH, Wetzlar, Germany).

3.3. Statistical Analysis {#sec3dot3-materials-10-00477}
-------------------------

The experimental data of mechanical and degradation properties were expressed as mean ± standard deviation. Statistical analysis was performed to assess the difference by the analysis of variance. The difference was considered to be significant when *p* \< 0.05.

4. Conclusions {#sec4-materials-10-00477}
==============

The microstructure, degradation properties and hardness of the AZ61 magnesium alloys with different Y contents (0, 1, 2, 3, 4 wt %) prepared by laser rapid melting were investigated. Adding Y to AZ61 magnesium alloy could lead to the formation of Al~2~Y phase and reduce the amount of Mg~17~Al~12~ phase. The degradation resistance of the AZ61 magnesium alloy was enhanced with Y addition. The AZ61 magnesium alloy with 2 wt % Y exhibited an optimal degradation resistance. Furthermore, the hardness increased as Y contents increased from 0 wt % to 2 wt %, and then decreased when Y contents decreased further. In conclusion, laser rapid melting AZ61 magnesium alloy with 2 wt % Y exhibit prospects for future bone implants.

This work was supported by the following funds: (1) The Natural Science Foundation of China (51575537, 81572577); (2) Hunan Provincial Natural Science Foundation of China (14JJ1006, 2016JJ1027); (3) The Project of Innovation-driven Plan of Central South University (2015CXS008, 2016CX023); (4) The Open-End Fund for the Valuable and Precision Instruments of Central South University; (5) The fund of the State Key Laboratory of Solidification Processing in NWPU (SKLSP201605); (6) The fund of the State Key Laboratory for Powder Metallurgy; (7)The Project of State Key Laboratory of High Performance Complex Manufacturing, Central South University.

Long Liu, Fulai Yuan and Cijun Shuai conceived and designed the experiments; Long Liu, Chengde Gao and Youwen Yang performed the experiments; Pei Feng and Sheng Yang analyzed the data; Mingchun Zhao contributed analysis tools; Long Liu and Fulai Yuan wrote the paper. All authors reviewed the final manuscript.

The authors declare no conflict of interest.

![Optical micrographs of AZ61 magnesium alloys with different Y contents: (**a**) 0 wt %; (**b**) 1 wt %; (**c**) 2 wt %; (**d**) 3 wt % and (**e**) 4 wt %.](materials-10-00477-g001){#materials-10-00477-f001}

![SEM micrographs of AZ61 magnesium alloys with different Y contents: (**a**) 0 wt %; (**b**) 1 wt %; (**c**) 2 wt %; (**d**) 3 wt % and (**e**) 4 wt %.](materials-10-00477-g002){#materials-10-00477-f002}

![X-ray diffraction (XRD) patterns of AZ61 magnesium alloys with different Y contents: (**a**) 0 wt %; (**b**) 1 wt %; (**c**) 2 wt %; (**d**) 3 wt % and (**e**) 4 wt %.](materials-10-00477-g003){#materials-10-00477-f003}

![The weight percent of Mg~17~Al~12~ and Al~2~Y phases in AZ61 magnesium alloys with Y addition.](materials-10-00477-g004){#materials-10-00477-f004}

![SEM image of (**a**) AZ61 magnesium alloy with 2 wt % Y and energy dispersive spectroscopy (EDS) patterns of (**b**) A line and (**c**) B point in (**a**).](materials-10-00477-g005){#materials-10-00477-f005}

![Schematic diagram of phase formation in the AZ61 magnesium alloy with Y (**a**) liquid phase; (**b**) Al~2~Y phase precipitation; (**c**) α-Mg nucleation; (**d**) Mg~17~Al~12~ formation.](materials-10-00477-g006){#materials-10-00477-f006}

![Hardness of AZ61 magnesium alloys with different Y contents.](materials-10-00477-g007){#materials-10-00477-f007}

![The hydrogen evolution volume of AZ61 magnesium alloys with different Y contents immersed in the simulated body fluid (SBF) for 360 h: (**a**) 0 wt %; (**b**) 1 wt %; (**c**) 2 wt %; (**d**) 3 wt % and (**e**) 4 wt %.](materials-10-00477-g008){#materials-10-00477-f008}

![Degradation rates of AZ61 magnesium alloys with different Y contents after immersion in SBF solution for 7 days.](materials-10-00477-g009){#materials-10-00477-f009}

![SEM degradation morphology of AZ61 magnesium alloys with different Y contents after immersion for 120 h: (**a**) 0 wt %; (**b**) 1 wt %; (**c**) 2 wt %; (**d**) 3 wt % and (**e**) 4 wt %.](materials-10-00477-g010){#materials-10-00477-f010}

[^1]: These authors contributed equally to this work.
